1st_assignment_solution

# 1st_assignment_solution - The University of Michigan...

• Notes
• 7
• 100% (1) 1 out of 1 people found this document helpful

This preview shows pages 1–3. Sign up to view the full content.

The University of Michigan - Dearborn Industrial and Manufacturing Systems Engineering Department IMSE 382: Manufacturing Processes I Assignment # 1 Mechanical Properties of Materials Solution 1. The following data were obtained during a tensile test of a standard specimen made of brass. D o = 12.50 mm, L o = 50.00 mm. Load and length readings are as follows: _ Load (N) Length (mm) Load (N) Length (mm) Load (N) Length (mm) 2,495 50.01 12,760 50.075 37,860 77.500 6,760 50.025 13,020 50.10 26,240 83.000 10,820 50.04 13,610 50.150 12,340 50.05 30,510 57.500 Ultimate Load = 42,090 N, and D f =6.25 mm, L f = 83.00. Determine the following: 1. Proof strength (using 0.2 % ) Load (N) Length (mm) A0 (mm^2) Eng Stress (MPa) Eng Strain True Stress (MPa) True Strain Comment 2,495 50.01 122.718438 20.33109328 0.0002 20.3351595 8.685E-05 6,760 50.025 122.718438 55.08544712 0.0005 55.11298985 0.00021709 10,820 50.04 122.718438 88.16931034 0.0008 88.23984579 0.0003473 12,340 50.05 122.718438 100.5553872 0.001 100.6559426 0.00043408 12,760 50.075 122.718438 103.9778558 0.0015 104.1338226 0.00065095 13,020 50.1 122.718438 106.0965269 0.002 106.3087199 0.00086772 13,610 50.15 122.718438 110.9042804 0.003 111.2369932 0.00130093 30,510 57.5 122.718438 248.6178982 0.15 285.9105829 0.06069784 42,090 122.718438 342.980247 Necking starts 37,860 77.5 122.718438 308.5110988 0.55 Unknown Unknown Unknown dia 26,240 83 122.718438 213.8228007 0.66 855.2912027 0.60205999 Use Df 1

This preview has intentionally blurred sections. Sign up to view the full version.

0 20 40 60 80 100 120 0 0.001 0.002 0.003 0.004 0.005 Engineering Strain Engineering Stress (MPa) From the above figure, proof strength 2245 111 MPa 2. Ultimate Tensile strength UTS = (Ultimate load)/A 0 = (42090)/122.72 = 343.0 MPa 3. Modulus of elasticity E = slope in the elastic region = (55.09 – 20.33) / (.0005 - .0002) = 115.9 GPa 4. Percentage elongation EL % = (Lf-L0)/Lo * 100 = (83 – 50)/50 *100 = 66 % 5. Modulus of toughness Toughness = area under the σ- ε curve 2245 2/3 * (UTS+YS) * EL = 2/3 * (343.0 + 111) * .66 = 199.8 MPa = 199.8 MJ / m 3 6. True stress true strain at ultimate load True Stress
This is the end of the preview. Sign up to access the rest of the document.
• Fall '10
• Tensile strength, true strain, Manufacturing Systems Engineering Department IMSE

{[ snackBarMessage ]}

### What students are saying

• As a current student on this bumpy collegiate pathway, I stumbled upon Course Hero, where I can find study resources for nearly all my courses, get online help from tutors 24/7, and even share my old projects, papers, and lecture notes with other students.

Kiran Temple University Fox School of Business ‘17, Course Hero Intern

• I cannot even describe how much Course Hero helped me this summer. It’s truly become something I can always rely on and help me. In the end, I was not only able to survive summer classes, but I was able to thrive thanks to Course Hero.

Dana University of Pennsylvania ‘17, Course Hero Intern

• The ability to access any university’s resources through Course Hero proved invaluable in my case. I was behind on Tulane coursework and actually used UCLA’s materials to help me move forward and get everything together on time.

Jill Tulane University ‘16, Course Hero Intern